# finite element method coupled with a numerical cellular

Embed Size (px)

TRANSCRIPT

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

residual stresses of dual phase DP600 steel Nd:YAG

laser welding

S. LIUa, A. GAVRUSb*, A. KOUADRI-HENNIc

a. Bretagne Loire University (UBL), INSA Rennes, LGCGM (EA 3913), 20 Avenue des

Buttes de Cöesmes, 35708, Rennes, France, email : [email protected]

b. Bretagne Loire University (UBL), INSA Rennes, LGCGM (EA 3913), 20 Avenue des

Buttes de Cöesmes, 35708, Rennes, France, email : [email protected]

c. Bretagne Loire University (UBL), INSA Rennes, LGCGM (EA 3913), 20 Avenue des

Buttes de Cöesmes, 35708, Rennes, France, email : [email protected]

Résumé :

Un modèle thermo-mécanique couplé séquentiellement a été développé pour étudier les contraintes

résiduelles de l'acier double phase DP600 soudé par un procédé au laser Nd: YAG. Un modèle

d'automate cellulaire numérique (CA) a d'abord été construit pour simuler l'évolution de la

microstructure lors d'un soudage au laser. Les résultats d'orientation de la microstructure CA obtenus

sont entrés dans un modèle d'éléments finis (FEM) pour décrire l’anisotropie élastique avec une loi

constitutive correspondante caractérisant le comportement thermo-mécanique du matériau en prenant

en compte l’écrouissage de la ferrite-martensite à double phase, la sensibilité à la température et

l'influence de la vitesse de déformation. L’analyse des contraintes résiduelles numériques prédites par

le modèle couplé CA-FEM montre une légère sensibilité à la vitesse de déformation.

Abstract :

A sequentially coupled thermo-mechanical model has been developed to investigate the residual

stresses of DP600 dual phase steel welded by a Nd:YAG laser process. A numerical cellular

automaton (CA) model has been firstly built to simulate the microstructure evolution during a laser

welding. The obtained CA microstructure orientation results are input into a finite element model

(FEM) to describe elasticity anisotropy together with a corresponding constitutive law characterizing

the thermo-mechanical material behavior taking into account the dual phase ferrite-martensite

hardening, the temperature sensitivity and the strain rate influence. Analysis of numerical residual

stresses predicted by the proposed coupled CA-FEM model show some influences of strain rate.

Key words : laser welding, dual phase DP600 steel, anisotropy, strain rate

sensitivity, residual stresses

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

1 Introduction

To reduce energy consumption and CO2 release, high strength alloy is widely used in automotive

industries to reduce the car weight [1]. Among the high strength low weight alloys, the dual-phase

(DP) steel possesses adequate ductility and high strength. DP600 contains about 15% hard martensite

in a soft ferrite matrix [2]. The body-centered-tetragonal martensite helps to improve the high strength

while the body-centered-cubic ferrite contributes to ductility [3]. The high strain-hardening rate can

increase absorption energy in car collision, thus helps to decrease damage [4]. As is seen in figure 1,

when the laser is focused on DP600 steel, the weld area absorbs energy rapidly and fused locally.

Three areas of Fusion Zone (FZ), Heat Affected Zone (HAZ) and Base Metal (BM) are used to stand

for different welding zone. The heated weld area expands but is compressed by the surrounding colder

area. If the obtained stress exceeds the low yield strength corresponding to high temperature of

material, the weld part is plastically hot-compressed. After cooling down, the weld part is too small

relative to surrounding colder part. Thus, laser welding usually produces tensile residual stresses on

the weld region and compressive residual stresses on the surrounding area. Many studies were

conducted on dual-phase DP600 steel behavior, however concerning welding simulation of residual

stresses there are not many precise material models for a numerical analysis. It is unclear how much

DP600 elastic and plastic material properties will influence the yield strength and consequently the

residual stresses of a laser welding simulation. Thus the main purpose of this study is to analyses more

precisely the DP600 thermo-mechanical constitutive model, especially in order to evaluate the

influence of the elastic and plastic anisotropy together with the strain rate sensitivity on simulated

welding residual stresses.

(a) (b) (c)

Figure 1. a) Laser welding process used by automotive industry [5]; b) The three laser welding zones

(FZ-Fusion Zone, HAZ-Heat Affected Zone, BM-Base Metal); c) FE results of thermal gradients

(FZ: grey part T > 1530°C, HAZ: from red to green part 25°C < T < 1530°C, BM: blue part T = 25°C)

2 CA Model – FEM Coupling

In the case of the deep penetration welding simulation, a conical heat source model with Gaussian

distribution is used and the thermal flux Qv is expressed from the laser power P and the efficiency

factor by: 2

9 Pe e Q ( , )=

c

r

r

23 ème

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

(2)

The shape of heat source, energy distribution and all variables of Eq. 1 and 2 are presented in figure 2.

Figure 2. Gauss heat distribution of a conical heat source

The geometry, mesh and boundary condition of the laser welding thermos-mechanical model are

pictured in figure 3. The path transversal to the weld line, the rolling direction and the directions of

residual stresses estimation are also illustrated. The angle between transversal path and rolling

direction is θ. A finite element model with 44160 C3D8R elements is selected for an Abaqus

numerical analysis where all the dimensions are defined according to experimental data.

(a) (b) (c)

Figure 3. Experimental plates welding and ABAQUS/FEM numerical model: a) experimental plate

welding along the rolling direction; b) Plates cut and welding patch using different orientations with

respect to the rolling direction; c) Geometry and boundary conditions

The flowchart of used CA-FEM coupled model to simulate the residual stresses is shown figure 4.

Based on the CA model the crystalline orientation and orientation fraction are firstly computed.

Starting from these data, using an initial estimation of martensitic elastic constants are computed the

corresponding weld orthotropic elastic constants used in a second step into the ABAQUS/FEM

simulation of the laser welding process to estimate the residual stresses distribution.

Figure 4. The flowchart of the CA-FE model used to simulate residual stresses

23 ème

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

3 Anisotropy of dual-phase DP600 steel

The anisotropy of dual phase DP600 steel has been analyzed both from the solidification process using

the numerical CA model and from the base metal thermo-mechanical behavior using a sequentially

coupled thermal-elastic-plastic model and a plane anisotropy theory. It is observed that the residual

stress longitudinal to welding direction is more influenced by the material anisotropy and the

temperature sensitivity. The analysis of a coupled anisotropy model consists to take into account the

anisotropy of weld and the anisotropy of base metal.

3.1 Analysis of weld elastic anisotropy

3.1.1 Base metal elasticity For a rigorous computation of the residual stresses, the thermo-elasticity properties of DP600 base

metal has an important influence, so the temperature influences are firstly considered to describe

variations of the Young’s modulus and Poisson’s ratio (Table 1).

Table 1. Young’s Modulus and Poisson’s ratio of DP600 steel

Temperature () 0 300 600 800

Young’s Modulus (GPa) 210 190 120 30

Poisson’s ratio 0.280 0.295 0.310 0.330

Thermal expansion coefficient 1.210 -5

1.510 -5

1.610 -5

1.610 -5

3.1.2 Weld material elasticity Because of the high cooling rate of laser welding, during the solidification process the face centered

cubic austenite of DP600 weld turns to body centered tetragonal martensite. This phase transformation

phenomenon has been observed by many previous experimental works [6,7]. Due to the phase

transformation and due to the the grain size decrease, the mechanical properties of the weld material

are changed, such as observed by measurements of micro-hardness [8,9]. N.Farabi et al. [10] have

investigated laser welding on DP600/DP980 steels and show that full martensite is found at FZ part

(Fusion Zone). In this work the elastic constants of DP600 weld martensite are assumed to be the

same with those of a martensitic steel [11]. If an orthotropic elastic anisotropy is considered, the

martensitic elastic compliance Sij which express the relationships between the elastic strain Voigth

vector and the Cauchy stress Voigth vector can be computed by:

(3)

Starting from results obtained in [11] the following values are taking into account to describe elastic

23 ème

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

ABAQUS software requires specifying the nine elastic engineering constants in the following

sequence: E1, E2, E3, ν12, ν13, ν23, G12, G13, G23. Using the crystallites orientations obtained by CA

computation, the martensite orthotropic elasticity of weld DP600 can be defined using specific

formula defining the influence of orientation angle. Thus the figure 5 pictures the crystalline growth

simulated by CA method. From the edge of the weld the crystallites pool gradually grow to the center

weld pool. Because these crystallites grow faster than the others along a preferential direction, starting

from the orientation’s distribution obtained by CA model, it can be observed that the preferred

orientation is around of = 37.54 with respect to the welding direction.

(a) 206 CA step (b) 721 CA step (c) 1774 CA step

Figure 5. Crystallites growth simulation obtained by the CA model

If the orthotropic elastic stiffness of original martensite in the initial coordinate system A is defined by

[Cij A ], the orthotropic elastic stiffness of the rotated martensite noted by [Cij

B ] corresponding to the

coordinate system B (defined by an orientation angle chosen in the plate plane) can be computed

from the following formulas:

(5)

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

(6)

The cosines components of the rotation matrix defining relationships between the x, y, z axis

coordinates of A xA, yA, zA and x, y, z axis coordinates of B xB, yB, zB are shown in table 2:

Table 2. Cosines values defining a plane rotation with the angle θ

xA yA zA

yB sin θ cos θ 0

zB 0 0 1

Concerning the temperature influence on all elastic constants firstly is considered a proportional

variation with the DP600 base metal Young’s modulus and Poisson’s modulus defined in table 1. A

linear interpolation is applied to decrease the elastic constants proportionally with the temperature

increases: 300, 600 and 800 using the following formulas:

(7)

Here WT stands the weld material Young’s Modulus and Poisson’s ratio values of E1, E2, E3, ν12, ν13,

ν23, G12, G13 and G23 at temperature T (0, 300, 600 and 800) and BT stands for the

corresponding base material Young’s Modulus and Poisson’s ratio values of Table 1.

Using the interpolation relationship (7) the elastic coefficients values corresponding to the original

martensitic compliance matrix [Sij A ] = [Cij

A ]

-1

are shown in Table 3.

Table 3. Elastic constants of weld material computed from Cij matrix of martensite (GPa)

T/ E1 E2 E3 υ12 υ13 Υ23 G12 G13 G23

0 203.40 203.07 202.72 0.2943 0.2902 0.2942 79.06 78.72 78.85

300 184.03 183.73 183.42 0.3101 0.3057 0.3100 71.53 71.22 71.34

600 116.23 116.04 115.84 0.3258 0.3213 0.3258 45.18 44.98 45.06

800 29.06 29.01 28.96 0.3469 0.3420 0.3468 11.29 11.25 11.26

Using formula (4), (5) and (6) it is computed the elastic compliance matrix corresponding to the

preferred crystallites orientation and all obtained parameters (Table 4) are input into the Abaqus FEM.

Table 4. Elastic constants of weld material computed from preferred crystallites orientation (GPa)

T/ E1 E2 E3 υ12 υ13 Υ23 G12 G13 G23

0 203.78 203.70 202.72 0.2924 0.2924 0.2935 78.93 78.85 78.85

300 184.37 183.30 183.42 0.3080 0.3081 0.3092 71.42 71.34 71.07

600 116.45 116.40 115.84 0.3237 0.3237 0.3249 45.10 45.05 44.88

800 29.11 29.10 28.96 0.3446 0.3446 0.3459 11.28 11.26 11.22

23 ème

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

3.2 Analysis of base metal plastic anisotropy

Based on experimental tensile tests and using formula of plane plastic anisotropic theory, Lankford

coefficients and Hill’s coefficients of DP600 base metal steel are presented in Table 5 [12]:

Table 5. Lankford coefficients and Hill parameters concerning DP600 base metal

r0 r45 r90 R11 R22 R33 R12 F G H N

1.0123 0.6487 0.9160 1 0.9748 0.9777 1.1172 0.5492 0.4969 0.5031 1.2017

4 Analysis of strain rate sensitivity

The hardening term H(p) of material plastic flow can only predict the rheological behavior at a

particular strain rate. For materials undergoing temperature variations a strain rate sensitivity analysis

must be add to predict more precisely the corresponding flow stress changes. The temperature

sensitivity F(T) under room temperature is set to 1 and a reference material strain rate is

chosen. Starting from the strain rate sensitivity function proposed by A. Gavrus [13,14]

physically based on kinetics of dislocations glide, available simultaneously for both static or dynamic

conditions and for materials undergoing important strain rate gradients, the below expression is used:

(8)

Concerning the dual-phase D600 steel the visco-plastic constitutive model can be written from general

rheological law of A. Gavrus [13,14] and previous work of S. Liu et al [12], considering an Avrami

mixture formulation based on plastic strain hardening of martensite, dynamic recovery of ferrite,

temperature influence and strain rate sensitivity using the following equation:

(9)

The hardening of martensite is described using a Ludwick law, the softening of ferritic phase is

described by a Voce model and the dual-phase mixture by a dynamic Avrami formulation. According

to the Eq. 9 and using the experimental true stress–plastic strain tensile data obtained at room

temperature (Figure 6), the corresponding identified parameters are presented in Table 6.

Table 6. Parameter identification results of DP600 plastic constitutive behavior at room temperature

0.2 331.74 2772.93 0.5765 621.08 11.5505

k m n p D

0.49 4.21 103.17 0.7023 1 0.0160537

*martensite fraction corresponding to the dual phase (ferrite-martensite) DP600 steel (here w=0.2)

It is shown from the flow stress curves plotted in figure 6 that the identified material plasticity model

of dual-phase DP600 steel predicts well the hardening and strain rate sensitivity.

23 ème

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

Figure 6. Comparison between experimental tensile flow stress curve at room temperature and the

identified thermo-mechanical plastic constitutive model

5 Numerical Results

Figure 7 plotted the equivalent residual stresses variation along the transversal path (see figure 3) for

the three material models: DP600 base metal model, weld model using material orientation along

welding direction and weld model using material orientations obtained by CA model. The mainly

difference between the three models is caused principally by the material elasticity properties. As is

described at section 3.1, DP600 base metal model use the reference metal elasticity for all material

zones (FZ, HAZ, BM), while the named weld model uses a weld material elasticity in the fusion

region (FZ). Nearly no differences are found on the residual stresses between the DP600 base model

and the weld model using orientations along welding direction. By introduction of weld material

orientations simulated by CA model, the numerical results on residual stresses are about 50 MPa

reduced around the weld zone. These results show that the difference of the elasticity considering

ferrite-martensite transition has little influence on residual stresses in numerical simulation of dual

phase steel DP600 laser welding. Moreover the elasticity differences considering crystals orientations

of weld material can reduce the residual stresses around the weld.

Figure 7. Numerical simulation results of Von-Mises residual stresses using three elasticity models

5.2 Analysis of base metal plastic anisotropy influence

Different plate welding orientations θ = 0°, 30°, 45°, 60° and 90°

with material rolling direction are

used to simulate welding process. The FEM numerical results concerning Hill’48 [15] equivalent

23 ème

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

residual stresses along transversal path are presented in figure 8. It can be observed that the material

rolling orientation influences the magnitude of equivalent Hill residual stresses around the weld.

Figure 8. Numerical Hill residual stresses obtained from different orientations of the welding with the

plate rolling direction

Equivalent stresses and effective plastic strains (PEEQ) distributions and corresponding values along

welding longitudinal and transversal path using FEM simulations with and without strain rate

sensitivity are compared and presented in figure 9 and 10. The numerical results show a general small

sensitivity of the strain rate term. However a particular important rise of the PEEQ and equivalent

residual stresses occur on the weld center area.

(a) (b)

Figure 9. Numerical iso-values of effective plastic strains (PEEQ) distribution: a) without strain rate

sensitivity term, b) with strain rate sensitivity term

(a) (b)

Figure 10. Numerical iso-values of Hill equivalent stress distribution: a) without strain rate sensitivity

term, b) with strain rate sensitivity term

23 ème

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

Furthermore comparisons of effective plastic strains variations pictured in figure 11 show that strain

rate sensitivity has little influence along a transversal welding path (with a maximum of 30% rise on

the welding center), but a relatively important effect (200%) particularly on the edge and middle part

along the longitudinal welding direction.

(a) (b)

Figure 11. Effective plastic strains (PEEQ) variations obtained by numerical simulations: a) along

transversal welding path, b) along longitudinal welding path

Concerning the Hill equivalent residual stresses variations along the transversal and longitudinal

welding path (figure 12) a little influence of the strain rate is again observed excepting the center

welding region where a difference around of 20% occurs.

(a) (b)

Figure 12. Hill equivalent residual stresses variations obtained by numerical simulations: a) along

transversal welding path, b) along longitudinal welding path

6 Conclusions

All the obtained numerical results of this study lead to a better understanding of the correlations

between the laser welding process and the welding microstructure, residual stresses and global weld

quality in the case of a dual-phase DP600 steel. The analysis of the proposed simulation model can

draw three major conclusions.

1. Concerning the influence of weld elastic anisotropy the equivalent residual stresses along

transversal path of base metal elasticity model and weld elasticity model have been compared.

23 ème

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

orientation influences the numerical residual stresses only in the central welding region.

2. Concerning the base metal plastic anisotropy influence, laser welding processes defined by

different orientations with respect to the material rolling have been simulated. The results of

equivalent residual stresses show that the plastic material anisotropy influence the magnitude of

longitudinal and transversal residual stresses around the weld.

3. To improve material plastic flow especially for a wide range of temperatures (from room

temperature to fusion temperature), a strain rate sensitivity model has been identified based on

experimental DP600 true stress-plastic strain tensile curves obtained at 20°C and on a modified

Johnson-Cook temperature sensitivity term. As a first approximation, the strain rate sensitivities

for high temperatures have been supposed in this work to be the same as that for room

temperature. It has been shown from the obtained numerical results of FEM simulations taking

into account a material strain rate constitutive behavior that the plastic strains and equivalent

residual stresses have similar global variations as compared with a FEM model without a strain

rate sensitivity term. However pronounced peaks with higher values were observed at the

beginning, center and end of the weld in the case of use of strain rate sensitivity.

Acknowledgement

The work was financially supported by China Scholarship Council and GCGM laboratory of INSA

Rennes.

References

[1] Geoffrey Davies, Materials for automobile bodies, Butterworth Heinemann, 2012.

[2] Marion Calcagnotto, Yoshitaka Adachi, Dirk Ponge, and Dierk Raabe, Deformation and

fracture mechanisms in fine-and ultrafine-grained ferrite/martensite dual-phase steels and the

effect of aging, Acta Materialia, 59(2) (2011) 658–670.

[3] Shuang Kuang, Yong-lin Kang, Hao Yu, and Ren-Dong Liu, Effect of continuous annealing

parameters on the mechanical properties and microstructures of a cold rolled dual phase steel,

International Journal of Minerals, Metallurgy and Materials 16(2) (2009) 159–164.

[4] O. Bouaziz, H. Zurob, and M. Huang, Driving force and logic of development of advanced high

strength steels for automotive applications. Steel Res. Int., 84(10) (2013) 937–947.

[5] Fraunhofer CLA, Making innovation a reality, Meet Fraunhofer IWS and Fraunhofer CCL’s

Laser Applications Division at LME.

[6] N. Farabi, D. L. Chen, J. Li, Y. Zhou, and S. J. Dong, Microstructure and mechanical properties

of laser welded dp600 steel joints, Materials Science and Engineering A 527(4–5) (2010) 1215–

1221.

[7] Danyang Dong, Yang Liu, Yuling Yang, Jinfeng Li, Min Ma, and Tao Jiang, Microstructure

and dynamic tensile behavior of DP600 dual phase steel joint by laser welding, Materials

Science and Engineering A 594 (2014) 17–25.

[8] Y Y Zhao, Y S Zhang, and W Hu, Effect of welding speed on microstructure, hardness and

tensile properties in laser welding of advanced high strength steel, Science and Technology of

Welding and Joining 18(7) (2013) 581–590.

23 ème

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

[9] Mingsheng Xia, Elliot Biro, Zhiling Tian, and Y. Norman Zhou, Effects of heat input and

martensite on haz softening in laser welding of dual phase steels, ISIJ International 48(6) (2008)

809–814.

[10] N. Farabi, D. L. Chen, and Y. Zhou, Microstructure and mechanical properties of laser welded

dissimilar dp600/dp980 dual-phase steel joints, J. of Alloys and Compounds 509(3) (2011)

982–989.

[11] Sudook A. Kim and Ward L. Johnson, Elastic constants and internal friction of martensitic

steel, ferritic-pearlitic steel, and α-iron, Mat. Sci. and Eng. A 452-453 (2007) 633–639.

[12] S. Liu, A. Kouadri-Henni, and A. Gavrus, Numerical simulation and experimental investigation

on the residual stresses in a laser beam welded dual phase DP600 steel plate: Thermo-

mechanical material plasticity model, Int. J. Mech. Sci. 243 (2017) 122:235.

[13] A. Gavrus, Formulation of a new constitutive equation available simultaneously for static and

dynamic loadings, DYMAT Int. Conf. on the Mechanical and Physical Behaviour of Materials

under Dynamic Loading, EDP Science, Bruxelles, Belgium, 2009, pp. 1239-1244.

[14] Adinel Gavrus, Constitutive equation for description of metallic materials behavior during static

and dynamic loadings taking into account important gradients of plastic deformation, Key

Engineering Materials 504 (2012) 697-702.

[15] Hill, R. A theory of the yielding and plastic flow of anisotropic metals. In: Proc. of the Royal

Septembre 2017

residual stresses of dual phase DP600 steel Nd:YAG

laser welding

S. LIUa, A. GAVRUSb*, A. KOUADRI-HENNIc

a. Bretagne Loire University (UBL), INSA Rennes, LGCGM (EA 3913), 20 Avenue des

Buttes de Cöesmes, 35708, Rennes, France, email : [email protected]

b. Bretagne Loire University (UBL), INSA Rennes, LGCGM (EA 3913), 20 Avenue des

Buttes de Cöesmes, 35708, Rennes, France, email : [email protected]

c. Bretagne Loire University (UBL), INSA Rennes, LGCGM (EA 3913), 20 Avenue des

Buttes de Cöesmes, 35708, Rennes, France, email : [email protected]

Résumé :

Un modèle thermo-mécanique couplé séquentiellement a été développé pour étudier les contraintes

résiduelles de l'acier double phase DP600 soudé par un procédé au laser Nd: YAG. Un modèle

d'automate cellulaire numérique (CA) a d'abord été construit pour simuler l'évolution de la

microstructure lors d'un soudage au laser. Les résultats d'orientation de la microstructure CA obtenus

sont entrés dans un modèle d'éléments finis (FEM) pour décrire l’anisotropie élastique avec une loi

constitutive correspondante caractérisant le comportement thermo-mécanique du matériau en prenant

en compte l’écrouissage de la ferrite-martensite à double phase, la sensibilité à la température et

l'influence de la vitesse de déformation. L’analyse des contraintes résiduelles numériques prédites par

le modèle couplé CA-FEM montre une légère sensibilité à la vitesse de déformation.

Abstract :

A sequentially coupled thermo-mechanical model has been developed to investigate the residual

stresses of DP600 dual phase steel welded by a Nd:YAG laser process. A numerical cellular

automaton (CA) model has been firstly built to simulate the microstructure evolution during a laser

welding. The obtained CA microstructure orientation results are input into a finite element model

(FEM) to describe elasticity anisotropy together with a corresponding constitutive law characterizing

the thermo-mechanical material behavior taking into account the dual phase ferrite-martensite

hardening, the temperature sensitivity and the strain rate influence. Analysis of numerical residual

stresses predicted by the proposed coupled CA-FEM model show some influences of strain rate.

Key words : laser welding, dual phase DP600 steel, anisotropy, strain rate

sensitivity, residual stresses

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

1 Introduction

To reduce energy consumption and CO2 release, high strength alloy is widely used in automotive

industries to reduce the car weight [1]. Among the high strength low weight alloys, the dual-phase

(DP) steel possesses adequate ductility and high strength. DP600 contains about 15% hard martensite

in a soft ferrite matrix [2]. The body-centered-tetragonal martensite helps to improve the high strength

while the body-centered-cubic ferrite contributes to ductility [3]. The high strain-hardening rate can

increase absorption energy in car collision, thus helps to decrease damage [4]. As is seen in figure 1,

when the laser is focused on DP600 steel, the weld area absorbs energy rapidly and fused locally.

Three areas of Fusion Zone (FZ), Heat Affected Zone (HAZ) and Base Metal (BM) are used to stand

for different welding zone. The heated weld area expands but is compressed by the surrounding colder

area. If the obtained stress exceeds the low yield strength corresponding to high temperature of

material, the weld part is plastically hot-compressed. After cooling down, the weld part is too small

relative to surrounding colder part. Thus, laser welding usually produces tensile residual stresses on

the weld region and compressive residual stresses on the surrounding area. Many studies were

conducted on dual-phase DP600 steel behavior, however concerning welding simulation of residual

stresses there are not many precise material models for a numerical analysis. It is unclear how much

DP600 elastic and plastic material properties will influence the yield strength and consequently the

residual stresses of a laser welding simulation. Thus the main purpose of this study is to analyses more

precisely the DP600 thermo-mechanical constitutive model, especially in order to evaluate the

influence of the elastic and plastic anisotropy together with the strain rate sensitivity on simulated

welding residual stresses.

(a) (b) (c)

Figure 1. a) Laser welding process used by automotive industry [5]; b) The three laser welding zones

(FZ-Fusion Zone, HAZ-Heat Affected Zone, BM-Base Metal); c) FE results of thermal gradients

(FZ: grey part T > 1530°C, HAZ: from red to green part 25°C < T < 1530°C, BM: blue part T = 25°C)

2 CA Model – FEM Coupling

In the case of the deep penetration welding simulation, a conical heat source model with Gaussian

distribution is used and the thermal flux Qv is expressed from the laser power P and the efficiency

factor by: 2

9 Pe e Q ( , )=

c

r

r

23 ème

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

(2)

The shape of heat source, energy distribution and all variables of Eq. 1 and 2 are presented in figure 2.

Figure 2. Gauss heat distribution of a conical heat source

The geometry, mesh and boundary condition of the laser welding thermos-mechanical model are

pictured in figure 3. The path transversal to the weld line, the rolling direction and the directions of

residual stresses estimation are also illustrated. The angle between transversal path and rolling

direction is θ. A finite element model with 44160 C3D8R elements is selected for an Abaqus

numerical analysis where all the dimensions are defined according to experimental data.

(a) (b) (c)

Figure 3. Experimental plates welding and ABAQUS/FEM numerical model: a) experimental plate

welding along the rolling direction; b) Plates cut and welding patch using different orientations with

respect to the rolling direction; c) Geometry and boundary conditions

The flowchart of used CA-FEM coupled model to simulate the residual stresses is shown figure 4.

Based on the CA model the crystalline orientation and orientation fraction are firstly computed.

Starting from these data, using an initial estimation of martensitic elastic constants are computed the

corresponding weld orthotropic elastic constants used in a second step into the ABAQUS/FEM

simulation of the laser welding process to estimate the residual stresses distribution.

Figure 4. The flowchart of the CA-FE model used to simulate residual stresses

23 ème

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

3 Anisotropy of dual-phase DP600 steel

The anisotropy of dual phase DP600 steel has been analyzed both from the solidification process using

the numerical CA model and from the base metal thermo-mechanical behavior using a sequentially

coupled thermal-elastic-plastic model and a plane anisotropy theory. It is observed that the residual

stress longitudinal to welding direction is more influenced by the material anisotropy and the

temperature sensitivity. The analysis of a coupled anisotropy model consists to take into account the

anisotropy of weld and the anisotropy of base metal.

3.1 Analysis of weld elastic anisotropy

3.1.1 Base metal elasticity For a rigorous computation of the residual stresses, the thermo-elasticity properties of DP600 base

metal has an important influence, so the temperature influences are firstly considered to describe

variations of the Young’s modulus and Poisson’s ratio (Table 1).

Table 1. Young’s Modulus and Poisson’s ratio of DP600 steel

Temperature () 0 300 600 800

Young’s Modulus (GPa) 210 190 120 30

Poisson’s ratio 0.280 0.295 0.310 0.330

Thermal expansion coefficient 1.210 -5

1.510 -5

1.610 -5

1.610 -5

3.1.2 Weld material elasticity Because of the high cooling rate of laser welding, during the solidification process the face centered

cubic austenite of DP600 weld turns to body centered tetragonal martensite. This phase transformation

phenomenon has been observed by many previous experimental works [6,7]. Due to the phase

transformation and due to the the grain size decrease, the mechanical properties of the weld material

are changed, such as observed by measurements of micro-hardness [8,9]. N.Farabi et al. [10] have

investigated laser welding on DP600/DP980 steels and show that full martensite is found at FZ part

(Fusion Zone). In this work the elastic constants of DP600 weld martensite are assumed to be the

same with those of a martensitic steel [11]. If an orthotropic elastic anisotropy is considered, the

martensitic elastic compliance Sij which express the relationships between the elastic strain Voigth

vector and the Cauchy stress Voigth vector can be computed by:

(3)

Starting from results obtained in [11] the following values are taking into account to describe elastic

23 ème

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

ABAQUS software requires specifying the nine elastic engineering constants in the following

sequence: E1, E2, E3, ν12, ν13, ν23, G12, G13, G23. Using the crystallites orientations obtained by CA

computation, the martensite orthotropic elasticity of weld DP600 can be defined using specific

formula defining the influence of orientation angle. Thus the figure 5 pictures the crystalline growth

simulated by CA method. From the edge of the weld the crystallites pool gradually grow to the center

weld pool. Because these crystallites grow faster than the others along a preferential direction, starting

from the orientation’s distribution obtained by CA model, it can be observed that the preferred

orientation is around of = 37.54 with respect to the welding direction.

(a) 206 CA step (b) 721 CA step (c) 1774 CA step

Figure 5. Crystallites growth simulation obtained by the CA model

If the orthotropic elastic stiffness of original martensite in the initial coordinate system A is defined by

[Cij A ], the orthotropic elastic stiffness of the rotated martensite noted by [Cij

B ] corresponding to the

coordinate system B (defined by an orientation angle chosen in the plate plane) can be computed

from the following formulas:

(5)

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

(6)

The cosines components of the rotation matrix defining relationships between the x, y, z axis

coordinates of A xA, yA, zA and x, y, z axis coordinates of B xB, yB, zB are shown in table 2:

Table 2. Cosines values defining a plane rotation with the angle θ

xA yA zA

yB sin θ cos θ 0

zB 0 0 1

Concerning the temperature influence on all elastic constants firstly is considered a proportional

variation with the DP600 base metal Young’s modulus and Poisson’s modulus defined in table 1. A

linear interpolation is applied to decrease the elastic constants proportionally with the temperature

increases: 300, 600 and 800 using the following formulas:

(7)

Here WT stands the weld material Young’s Modulus and Poisson’s ratio values of E1, E2, E3, ν12, ν13,

ν23, G12, G13 and G23 at temperature T (0, 300, 600 and 800) and BT stands for the

corresponding base material Young’s Modulus and Poisson’s ratio values of Table 1.

Using the interpolation relationship (7) the elastic coefficients values corresponding to the original

martensitic compliance matrix [Sij A ] = [Cij

A ]

-1

are shown in Table 3.

Table 3. Elastic constants of weld material computed from Cij matrix of martensite (GPa)

T/ E1 E2 E3 υ12 υ13 Υ23 G12 G13 G23

0 203.40 203.07 202.72 0.2943 0.2902 0.2942 79.06 78.72 78.85

300 184.03 183.73 183.42 0.3101 0.3057 0.3100 71.53 71.22 71.34

600 116.23 116.04 115.84 0.3258 0.3213 0.3258 45.18 44.98 45.06

800 29.06 29.01 28.96 0.3469 0.3420 0.3468 11.29 11.25 11.26

Using formula (4), (5) and (6) it is computed the elastic compliance matrix corresponding to the

preferred crystallites orientation and all obtained parameters (Table 4) are input into the Abaqus FEM.

Table 4. Elastic constants of weld material computed from preferred crystallites orientation (GPa)

T/ E1 E2 E3 υ12 υ13 Υ23 G12 G13 G23

0 203.78 203.70 202.72 0.2924 0.2924 0.2935 78.93 78.85 78.85

300 184.37 183.30 183.42 0.3080 0.3081 0.3092 71.42 71.34 71.07

600 116.45 116.40 115.84 0.3237 0.3237 0.3249 45.10 45.05 44.88

800 29.11 29.10 28.96 0.3446 0.3446 0.3459 11.28 11.26 11.22

23 ème

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

3.2 Analysis of base metal plastic anisotropy

Based on experimental tensile tests and using formula of plane plastic anisotropic theory, Lankford

coefficients and Hill’s coefficients of DP600 base metal steel are presented in Table 5 [12]:

Table 5. Lankford coefficients and Hill parameters concerning DP600 base metal

r0 r45 r90 R11 R22 R33 R12 F G H N

1.0123 0.6487 0.9160 1 0.9748 0.9777 1.1172 0.5492 0.4969 0.5031 1.2017

4 Analysis of strain rate sensitivity

The hardening term H(p) of material plastic flow can only predict the rheological behavior at a

particular strain rate. For materials undergoing temperature variations a strain rate sensitivity analysis

must be add to predict more precisely the corresponding flow stress changes. The temperature

sensitivity F(T) under room temperature is set to 1 and a reference material strain rate is

chosen. Starting from the strain rate sensitivity function proposed by A. Gavrus [13,14]

physically based on kinetics of dislocations glide, available simultaneously for both static or dynamic

conditions and for materials undergoing important strain rate gradients, the below expression is used:

(8)

Concerning the dual-phase D600 steel the visco-plastic constitutive model can be written from general

rheological law of A. Gavrus [13,14] and previous work of S. Liu et al [12], considering an Avrami

mixture formulation based on plastic strain hardening of martensite, dynamic recovery of ferrite,

temperature influence and strain rate sensitivity using the following equation:

(9)

The hardening of martensite is described using a Ludwick law, the softening of ferritic phase is

described by a Voce model and the dual-phase mixture by a dynamic Avrami formulation. According

to the Eq. 9 and using the experimental true stress–plastic strain tensile data obtained at room

temperature (Figure 6), the corresponding identified parameters are presented in Table 6.

Table 6. Parameter identification results of DP600 plastic constitutive behavior at room temperature

0.2 331.74 2772.93 0.5765 621.08 11.5505

k m n p D

0.49 4.21 103.17 0.7023 1 0.0160537

*martensite fraction corresponding to the dual phase (ferrite-martensite) DP600 steel (here w=0.2)

It is shown from the flow stress curves plotted in figure 6 that the identified material plasticity model

of dual-phase DP600 steel predicts well the hardening and strain rate sensitivity.

23 ème

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

Figure 6. Comparison between experimental tensile flow stress curve at room temperature and the

identified thermo-mechanical plastic constitutive model

5 Numerical Results

Figure 7 plotted the equivalent residual stresses variation along the transversal path (see figure 3) for

the three material models: DP600 base metal model, weld model using material orientation along

welding direction and weld model using material orientations obtained by CA model. The mainly

difference between the three models is caused principally by the material elasticity properties. As is

described at section 3.1, DP600 base metal model use the reference metal elasticity for all material

zones (FZ, HAZ, BM), while the named weld model uses a weld material elasticity in the fusion

region (FZ). Nearly no differences are found on the residual stresses between the DP600 base model

and the weld model using orientations along welding direction. By introduction of weld material

orientations simulated by CA model, the numerical results on residual stresses are about 50 MPa

reduced around the weld zone. These results show that the difference of the elasticity considering

ferrite-martensite transition has little influence on residual stresses in numerical simulation of dual

phase steel DP600 laser welding. Moreover the elasticity differences considering crystals orientations

of weld material can reduce the residual stresses around the weld.

Figure 7. Numerical simulation results of Von-Mises residual stresses using three elasticity models

5.2 Analysis of base metal plastic anisotropy influence

Different plate welding orientations θ = 0°, 30°, 45°, 60° and 90°

with material rolling direction are

used to simulate welding process. The FEM numerical results concerning Hill’48 [15] equivalent

23 ème

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

residual stresses along transversal path are presented in figure 8. It can be observed that the material

rolling orientation influences the magnitude of equivalent Hill residual stresses around the weld.

Figure 8. Numerical Hill residual stresses obtained from different orientations of the welding with the

plate rolling direction

Equivalent stresses and effective plastic strains (PEEQ) distributions and corresponding values along

welding longitudinal and transversal path using FEM simulations with and without strain rate

sensitivity are compared and presented in figure 9 and 10. The numerical results show a general small

sensitivity of the strain rate term. However a particular important rise of the PEEQ and equivalent

residual stresses occur on the weld center area.

(a) (b)

Figure 9. Numerical iso-values of effective plastic strains (PEEQ) distribution: a) without strain rate

sensitivity term, b) with strain rate sensitivity term

(a) (b)

Figure 10. Numerical iso-values of Hill equivalent stress distribution: a) without strain rate sensitivity

term, b) with strain rate sensitivity term

23 ème

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

Furthermore comparisons of effective plastic strains variations pictured in figure 11 show that strain

rate sensitivity has little influence along a transversal welding path (with a maximum of 30% rise on

the welding center), but a relatively important effect (200%) particularly on the edge and middle part

along the longitudinal welding direction.

(a) (b)

Figure 11. Effective plastic strains (PEEQ) variations obtained by numerical simulations: a) along

transversal welding path, b) along longitudinal welding path

Concerning the Hill equivalent residual stresses variations along the transversal and longitudinal

welding path (figure 12) a little influence of the strain rate is again observed excepting the center

welding region where a difference around of 20% occurs.

(a) (b)

Figure 12. Hill equivalent residual stresses variations obtained by numerical simulations: a) along

transversal welding path, b) along longitudinal welding path

6 Conclusions

All the obtained numerical results of this study lead to a better understanding of the correlations

between the laser welding process and the welding microstructure, residual stresses and global weld

quality in the case of a dual-phase DP600 steel. The analysis of the proposed simulation model can

draw three major conclusions.

1. Concerning the influence of weld elastic anisotropy the equivalent residual stresses along

transversal path of base metal elasticity model and weld elasticity model have been compared.

23 ème

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

orientation influences the numerical residual stresses only in the central welding region.

2. Concerning the base metal plastic anisotropy influence, laser welding processes defined by

different orientations with respect to the material rolling have been simulated. The results of

equivalent residual stresses show that the plastic material anisotropy influence the magnitude of

longitudinal and transversal residual stresses around the weld.

3. To improve material plastic flow especially for a wide range of temperatures (from room

temperature to fusion temperature), a strain rate sensitivity model has been identified based on

experimental DP600 true stress-plastic strain tensile curves obtained at 20°C and on a modified

Johnson-Cook temperature sensitivity term. As a first approximation, the strain rate sensitivities

for high temperatures have been supposed in this work to be the same as that for room

temperature. It has been shown from the obtained numerical results of FEM simulations taking

into account a material strain rate constitutive behavior that the plastic strains and equivalent

residual stresses have similar global variations as compared with a FEM model without a strain

rate sensitivity term. However pronounced peaks with higher values were observed at the

beginning, center and end of the weld in the case of use of strain rate sensitivity.

Acknowledgement

The work was financially supported by China Scholarship Council and GCGM laboratory of INSA

Rennes.

References

[1] Geoffrey Davies, Materials for automobile bodies, Butterworth Heinemann, 2012.

[2] Marion Calcagnotto, Yoshitaka Adachi, Dirk Ponge, and Dierk Raabe, Deformation and

fracture mechanisms in fine-and ultrafine-grained ferrite/martensite dual-phase steels and the

effect of aging, Acta Materialia, 59(2) (2011) 658–670.

[3] Shuang Kuang, Yong-lin Kang, Hao Yu, and Ren-Dong Liu, Effect of continuous annealing

parameters on the mechanical properties and microstructures of a cold rolled dual phase steel,

International Journal of Minerals, Metallurgy and Materials 16(2) (2009) 159–164.

[4] O. Bouaziz, H. Zurob, and M. Huang, Driving force and logic of development of advanced high

strength steels for automotive applications. Steel Res. Int., 84(10) (2013) 937–947.

[5] Fraunhofer CLA, Making innovation a reality, Meet Fraunhofer IWS and Fraunhofer CCL’s

Laser Applications Division at LME.

[6] N. Farabi, D. L. Chen, J. Li, Y. Zhou, and S. J. Dong, Microstructure and mechanical properties

of laser welded dp600 steel joints, Materials Science and Engineering A 527(4–5) (2010) 1215–

1221.

[7] Danyang Dong, Yang Liu, Yuling Yang, Jinfeng Li, Min Ma, and Tao Jiang, Microstructure

and dynamic tensile behavior of DP600 dual phase steel joint by laser welding, Materials

Science and Engineering A 594 (2014) 17–25.

[8] Y Y Zhao, Y S Zhang, and W Hu, Effect of welding speed on microstructure, hardness and

tensile properties in laser welding of advanced high strength steel, Science and Technology of

Welding and Joining 18(7) (2013) 581–590.

23 ème

Congrès Français de Mécanique Lille, 28 Août au 1 er

Septembre 2017

[9] Mingsheng Xia, Elliot Biro, Zhiling Tian, and Y. Norman Zhou, Effects of heat input and

martensite on haz softening in laser welding of dual phase steels, ISIJ International 48(6) (2008)

809–814.

[10] N. Farabi, D. L. Chen, and Y. Zhou, Microstructure and mechanical properties of laser welded

dissimilar dp600/dp980 dual-phase steel joints, J. of Alloys and Compounds 509(3) (2011)

982–989.

[11] Sudook A. Kim and Ward L. Johnson, Elastic constants and internal friction of martensitic

steel, ferritic-pearlitic steel, and α-iron, Mat. Sci. and Eng. A 452-453 (2007) 633–639.

[12] S. Liu, A. Kouadri-Henni, and A. Gavrus, Numerical simulation and experimental investigation

on the residual stresses in a laser beam welded dual phase DP600 steel plate: Thermo-

mechanical material plasticity model, Int. J. Mech. Sci. 243 (2017) 122:235.

[13] A. Gavrus, Formulation of a new constitutive equation available simultaneously for static and

dynamic loadings, DYMAT Int. Conf. on the Mechanical and Physical Behaviour of Materials

under Dynamic Loading, EDP Science, Bruxelles, Belgium, 2009, pp. 1239-1244.

[14] Adinel Gavrus, Constitutive equation for description of metallic materials behavior during static

and dynamic loadings taking into account important gradients of plastic deformation, Key

Engineering Materials 504 (2012) 697-702.

[15] Hill, R. A theory of the yielding and plastic flow of anisotropic metals. In: Proc. of the Royal